Characterisation and categorisation of the diversity
in viscoelastic vibrational properties between 98 wood typesIris Brémaud&Yves El Kaïm&Daniel Guibal&
Kazuya Minato&Bernard Thibaut&Joseph Gril
Received: 18 August 2011 / Accepted: 15 November 2011 / Published online: 9 December 2011 # INRA / Springer-Verlag France 2011
&Context Increased knowledge on diversity in wood proper-ties would have implications both for fundamental research and for promoting a diversification of uses as material.
& Aims The objective is to contribute to overcoming the critical lack of data on the diversity of wood dynamic mechanical/viscoelastic vibrational properties by testing lesser known species and categorising sources of variability.
& Methods Air-dry axial specific dynamic modulus of elasticity (E′/γ) and damping coefficient (tanδ) were measured on a wide sampling (1,792 specimens) of 98 wood types from 79 species. An experimental device and protocol was designed for conducting systematic (i.e. rapid and reproducible) characterisations.
& Results Diversity at the specimens’ level corroborates the “standard” relationship between tanδ and E′/γ, which is discussed in terms of orientation of wood elements and of chemical composition. Diversity at the species level is expressed on the basis of results for normal heartwood, with specific gravity (γ) ranging from 0.2 to 1.3. Axial E′/γ ranges from 9 to 32 GPa and tanδ from 4×10−3to 19×10−3. Properties distribution follows a continuum, but with group characteristics. The lowest values of tanδ are only found in certain tropical hardwoods. Results can also suggest alternative species for musical instruments making.
& Conclusion The variations in specific gravity, in stiffness or in “viscosity” appear to be predominantly linked to different levels of diversity: between species or between wood types (reaction wood or taxonomy-related differences in heartwood extractives).
Keywords Damping coefficient . Dynamic mechanical properties . Specific dynamic modulus of elasticity . Specific gravity . Viscoelastic vibrational properties . Wood diversity
Exploring the diversity of wood properties has long been a goal of foresters and wood technologists and more recently has found implications in research into functional ecology and biomechanics (e.g. Chave et al. 2009). Large databases of physico-mechanical properties can also contribute to a
Handling Editor: Barry Alan Gardiner
Contribution of co-authors I.B. designed and performed research and wrote the paper; Y.E.K. realized test device II and control/ processing software; D.G. did physical tests; K.M. initiated the methodology; K.M., B.T. and J.G. supervised the work and edited the paper.
:Y. El Kaïm
Laboratoire de Mécanique et Génie Civil (LMGC), CNRS, Université Montpellier 2, Place E. Bataillon, cc 048, 34095 Montpellier cedex 5, France
Laboratory of Forest Resources Circulatory System, Kyoto Prefectural University,
Kyoto 606-8522, Japan D. Guibal
UPR Production et Valorisation des Bois Tropicaux et Méditerranéens, CIRAD,
BP 5035, 34398 Montpellier cedex 5, France B. Thibaut
UMR Ecologie des Forêts de Guyane, CNRS, BP 316-97379 Kourou cedex, French Guyana, France Present Address:
I. Brémaud (*)
Wood Laboratory, EMPA,
Überlandstrasse 129, 8600 Dübendorf, Switzerland e-mail: email@example.com
physical understanding of traditional preferences for specific woods in various cultural uses (Brémaud 2012). They are also the pre-requisite for applying material selection methods (e.g. Wegst 2006), which could allow more efficient, diversified and potentially sustainable utilisation of wood materials. Amongst the 50,000+ wood-producing species, data are available for a proportionally moderate, yet quite important number of species for some properties: at least 8,000 species for specific gravity or density (e.g. Détienne and Chanson1996; Chave et al.2009), a minimum of 1,000– 2,000 species for the longitudinal modulus of elasticity (unpublished database at CIRAD; many other wood technol-ogy resources). Unfortunately, there is still a critical lack of knowledge on the diversity of some other relevant properties, notably concerning anisotropy and viscoelasticity. An up-to-date census on most published data on viscoelastic vibrational properties reveals that≤400 species have been characterised, even partially (Brémaud et al.2009; Brémaud2012).
The diversity in wood properties expresses variations in structure (cellular and sub-cellular) and chemical composi-tion (constitutive polymers and secondary metabolites). For wood along the grain, cellular anatomy mostly intervenes in the sense of “porosity”, i.e. it determines specific gravity (γ) and thus affects Young’s modulus (E). On the contrary, vibrational properties (specific dynamic modulus of elas-ticity=E′/γ and damping coefficient=tanδ) are primarily governed at the cell-wall level, with E′/γ decreasing, and tanδ increasing, with increasing microfibril angle (Obataya et al. 2000). As a result, a strong relationship generally exists between tanδ and E′/γ (Ono and Norimoto 1983, 1984). Variations in grain angle have similar impacts on both properties and result in a comparable tanδ–E′/γ relationship (Brémaud et al. 2010a, 2011b). Futhermore, the composition of the “matrix” of hemicelluloses and lignin determines the viscous behaviour (Obataya et al. 2000; Olsson and Salmén 1992, 1997). Some extractive compounds can also play a key role in modifying tanδ, by as much as a factor 2, with only minor effects on E′/γ (Yano 1994; Matsunaga et al. 1996; Obataya et al.1999; Minato et al.2010; Brémaud et al.2010b,2011a).
Anatomical and chemical features can be related to or even be characteristic of various levels of diversity, from plant order to species, and also be related to biogeography. Softwoods generally have a simpler anatomy and a higher content of lignin, which also has a more condensed chemical structure (Olsson and Salmén 1992, 1997). Amongst hardwoods, tropical ones show more diversity and often some typical features such as interlocked grain or high extractives content (EC) (e.g. Hernandez 2007; Brémaud et al.2010a,b). Cellular anatomy and secondary metabolites can be particularly characteristic of a genus or even a species. In addition to species diversity, there is a wide within-species variability, between or within trees,
between different wood types, e.g.“normal” versus reaction wood (variations in both anatomy and polymers), or heartwood versus sapwood (variations in extractives but similar anatomy and constitutive polymers).
The exploration and analysis of the diversity in wood properties requires obtaining very large datasets. A few long-term studies using the same methodology exist (e.g. Détienne and Chanson1996; unpublished CIRAD database and other research institutes resources). In order to compare a maximum of species, however, results from different sources have to be compiled (e.g. Chave et al. 2009; Brémaud et al. 2009). This efficient approach has never-theless drawbacks: even in the case of“simple” properties such as specific gravity or density, comparison of data obtained by different methodologies can be misleading (Williamson and Wiemann 2010). For viscoelastic vibra-tional properties, many sources (mainly Japanese) have employed non-contact forced vibrations of free-free (i.e., freely supported) beams (e.g. Fukada 1950; Obataya et al. 2000). Comparison of results on well-known or“reference” species across several sources supports the reproducibility potential of this method (e.g. analyses of the database described in Brémaud et al. 2009; Brémaud2012).
The general objective of this work is to increase knowledge on the diversity of wood dynamic mechanical/ viscoelastic vibrational properties. In a previous article, physico-chemical indicators were proposed for estimating variations in damping coefficient (Brémaud et al. 2010b). The present paper aims at producing new and reliable data on lesser known species and at categorising sources of variations. An attempt is also made at confronting species diversity and within-species variability. Ninety-eight con-trasting wood types, of which 65 had never been tested previously, are characterised. Potential sources of experi-mental errors are briefly reviewed, and a device and protocol are described for conducting systematic and rapid “routine” tests. Results are analysed at the specimen, wood type and species level. Repartition of properties between wood types is discussed in connection to their origin and to actual or potential acoustical end-uses.
2 Materials and methods
2.1 Wood material
Material was chosen in order to cover: (1) a wide range in botanical origins, specific gravity and extractives content; (2) both “reference” species for which data are available and species for which vibrational properties had never been studied; and (3) a range of actual or potential acoustical end-uses. Seventy-nine species were studied in total. In order to confront species diversity and within-species variability,
different wood types (WT) were collected for some species (e. g. heartwood versus sapwood or reaction versus normal wood). The sampling covered 98 WT: 19 (from 12 species) for softwoods, 14 (12 spp.) for temperate-zone hardwoods and 65 (55 spp.) for tropical hardwoods. It comprised of 264 stocks of wood, e.g. different trees and/or different“qualities”. Part of the wood material was obtained from the well-identified stocks from the CIRAD wood workshop. Another part was provided by several French instrument makers, and, when needed, botanical species were subsequently identified.
2.2 Sampling, scaling and preparation of test specimens
Specimens were cut to dimensions of 150×12×2 mm3 (longitudinal×radial×tangential), using a circular saw with a quality finishing blade and a specific machining guide and fixture. This procedure ensured smooth surfaces that did not require further processing (such as hand sanding, which would be detrimental to the parallelism of the specimen). Thickness variations were ≤0.05 mm. The total number of specimens was 1,792.
The quality of the specimens’ machining is of utmost importance. The accuracy of the thickness is the main source of experimental uncertainty on the specific modulus of elasticity (E′/γ). Damage in the surface layers, such as those resulting from machine planing, belt sanding or milling, must be avoided, as they reduce the modulus of elasticity and increase the damping (Sali and Kopac1998).
The sampling and scaling of specimens was carefully planned regarding local variations in wood. The width of specimens included at least one full growth ring—when these were distinct. Systematic grain angle deviations often cannot be avoided, especially so in tropical hardwoods, but they were carefully recorded, given their important effect on vibrational properties (Brémaud et al.2010a,2011b).
The slenderness (length/height ratio) of specimens is very important. In bending vibration, the total deflection includes a contribution of shear properties, which increases with reduc-ing slenderness, with increasreduc-ing anisotropy and with increas-ing order of vibration modes and frequency (Ono and Kataoka 1979; Obataya et al. 2000). This effect can be calculated (Nakao et al. 1985; Brancheriau and Baillères 2002; Kubojima et al. 2004), taking into account the range in axial-to-shear anisotropy of vibrational properties between very different woods (Brémaud et al.2011b). For E′ not to be under-evaluated by more than 2% (by Euler–Bernouilli Eq.1, at the first bending mode), the minimum l/h ratio is of the order of 25–40 for woods within the low to high range of anisotropy respectively. For tanδ (at the first bending mode), the contribution of shear remains under 2% for l/ h ratios >20 and can be neglected for l/h ratios >35. With the usual geometry (l/h=75) of specimens under study, the contribution of shear should be negligible at the first bending
mode, whatever the wood type. Slenderness should also be designed so that specimen stiffness is not excessive to allow precise displacement measurements.
2.3 Physical conditions
Before being tested, all specimens were conditioned for at least 3 weeks in standard “air-dry” regulated conditions (20 ± 1°C and 60–65% relative humidity RH). Equilibrium moisture content (EMC, calculated from measured “air-dry” weight and after oven-drying) ranged between 6% and 12% depending on species. Differences in EMC were primarily related to those in extractives content (Brémaud et al. 2010b). According to Obataya et al. (1998), a variation in EMC from 6% to 12% in a given wood (spruce) conditioned at different RH would result in a decrease in E′/γ of approximately −6% and an increase in tanδ of approximately 24%. However, woods with various chemical contents can exhibit differ-ent moisture contdiffer-ent dependence of vibrational properties (Obataya and Norimoto1995; Obataya et al.2001).
For practical reasons, part of the tests could not be run in the climate chamber but with an uncontrolled RH of 55– 65%. Variations in MC during the time of the tests were, however, quite small (≤3% relative variation, corresponding to ≤0.3% absolute change) and we could not detect significant short-term (~30 min) variation in E′/γ nor in tanδ. A sub-sample of 55 specimens, covering a wide range of properties, was tested in both conditions (inside and outside a climatic room) and measured values were identical on average. This, however, should not hold true if bigger differences in RH were considered.
2.4 Non-contact forced-released flexural vibrations of free-free beams
2.4.1 Basic principle
Slender wooden beams are hung by thin threads located at the nodes of vibration of the mode under study (here, the first mode). The specimen is made to vibrate through an electro-magnet facing a thin steel piece glued to one end of the sample. A frequency sweep detects the resonance frequency, from which the specific dynamic modulus of elasticity is determined according to the Euler–Bernouilli equation: E0 r ¼ 48p2l4 m4 nh2 fRn2 ð1Þ
where l is the length of the specimen and h its thickness, fRnis the resonance frequency of the mode n and mnis a constant depending on the mode order (m1=4.730). The specific modulus is expressed as E′/ρ in MPa m3
when using density (ρ, i.e. specific mass in kg m−3) or as E′/γ in GPa when using specific gravity (γ, without unit).
The damping coefficient (or loss factor, tanδ) is determined, in the time-domain, through the logarithmic decrement (λ=πtanδ, Fig.1b) of amplitudes, after stopping the excitation, which is fixed at fR. In the frequency domain, tanδ is determined by a frequency scan, through the bandwidth (Δf) at half-power (or at −3 dB) of the resonance curve (Fig. 1a), often called the quality factor (Q−1=Δf/fR). Both measurements should be equivalent (tanδ≈Q−1≈λ/π) for values <<0.1 (Jones2001).
2.4.2 Experimental devices and development of a semi-automated interface
The first used device employed an eddy-current displace-ment sensor (5 μm resolution, distance of detection 2± 0.2 mm), facing a thin aluminium plate glued on one end of the specimen (Fig. 2). The frequency scan was imposed manually from a function generator. The resonance fre-quency (fR) and the decrement of amplitude after stopping the excitation were recorded with a fast Fourier transform (FFT) analyser, and the data files were later analysed in MS Excel. The logarithmic decrement (λ, Fig. 1b) was determined by a regression on the peak amplitudes versus time. One triplicate test required≥15 min.
A more automated device was then designed in order to minimise the time required for a test and all manual steps (Brémaud 2006). Displacement was measured by a laser-triangulation sensor (Fig. 2), which simplifies positioning of specimens (10μm resolution, distance of detection 40± 4 mm). Tests were fully computer-driven through a control/ acquisition card (National Instruments, Austin, TX, USA, NI PCI 6221, A/D conversion 16 bits) and a program that we specifically developed in Labview®, with the following steps (Fig.3). A wide (150–750 Hz by default, adjustable) scan detected the first resonance frequency fR. Then, a narrower (0.98×fR−1.02×fR by default, adjustable) fre-quency sweep was run for measuring precisely (±0.05 Hz) fRand the bandwidth at half-power (Δf). The sampling rate was of 100 kS/s, and the acquisition time, by default, was 10 s. The signal (convoluted by a sine cardinal function as a
“natural” window is used in order not to modify the bandwidth) was smoothed by a moving average (on 5 points), on which fRandΔf were determined. Vibration was then set at fRuntil the vibration was stable and stopped. The logarithmic decrement (λ) after stopping the excitation was calculated by a regression on the peak amplitudes versus time on the steadiest part of the decay. The time required for measuring fR, tanδ=Q−1 and tanδ=λ/π of a specimen, with three repetitions, was≤5 min.
2.5 Validation of the experimental method
2.5.1 Calculated uncertainty and observed repeatability
The theoretical uncertainty on E′/γ is 5.9% (due to machining precision on thickness), and variations between repetitions were <1%.
For the determination of damping by bandwidth (Q−1), the calculated uncertainty is governed by the frequency resolution, that is, by the sampling rate and duration of acquisition. Uncertainty will be between 2.5% and 5% at 100 kS/s over 10 s (or twice higher values if using a sampling rate of 50 kS/s), for realistic ranges of Q−1values for wood. For tanδ determined by logarithmic decrement, the theoretical uncertainty depends on the initial amplitude of vibration and on the spatial resolution of the displace-ment sensor. In our experidisplace-mental conditions, it ranges from 1% to 15% (resolutions of 5 and 10μm). Measurements by bandwidth (tanδ=Q−1) have a lower relative uncertainty for woods with higher tanδ, whereas those by logarithmic decrement (tanδ=λ/π) have a lower relative uncertainty for woods with lower tanδ.
These calculated errors were closely matched by observed variations between repetitions (Fig. 4). Average experimental error was 3% for the bandwidth method and 5% (sensor resolution of 10 μm) or 2% (5 μm) by the logarithmic decrement method. For the latter, however, out-of-range values were observed for specimens with exces-sive stiffness and/or irregular surfaces. Nevertheless, the precision of tanδ determination in the temporal domain could be greatly improved using a simple“inverse” method (Fig. 1c). In this case, tanδ was identified over the whole
Fig. 1 Determination of tanδ in the frequency (a) or temporal (b, c) domains. a Bandwidth method; b logarithmic decrement method; c “inverse” method
signal (not only peak amplitudes) by fitting the parameters of the equation of decay (Fig.1c) to the experimental signal by optimisation (using the solver in MS Excel) so as to minimise the difference between the calculation and observations. Error was then normally ≤2% and did not exceed 5% even for“odd” specimens (Fig. 4).
Globally, the experimental error on tanδ ranged from 0% to 15.2% (mean=3.2%) and was≤5% for 80% of all tested specimens.
2.5.2 Comparison of measurements obtained by different methods
The values of tanδ determined in both the temporal and frequency domains (with the developed semi-automated device) were very consistent (Fig.5). This is in agreement with the theory of viscoelastic damping (Jones2001) and confirms its validity over the expectable range of axial tanδ for “air-dry” wood. Measurements by bandwidth were on average slightly higher (≈+0.4%) due to the modulation of the resonance peak by the observation window.
In bending vibration tests, the specific dynamic modulus of elasticity can be derived according to either Euler– Bernouilli (in which the influence of shear is neglected) or to the Timoshenko theory (which takes into account the influence of shear) (e.g. Brancheriau and Baillères2002). In order to compare the respective values obtained for E′/γ,
tests were conducted with a natural vibration method, which allows both calculations (without inputting hypo-thetical values for shear; Bordonné 1989). A reduced sampling of 130 beams, with dimensions 360 × 20 × 20 mm3 (L×R×T), were put into bending vibrations by percussion and their response (resonance frequencies of the three first bending modes) was recorded with a microphone. Beams were then cut into small specimens (2–6 per bar), which were tested by the forced vibration method.
For the same “bulk” specimens (20×20 mm section, l/h ratio of 18), E′/γ calculated according to Bernouilli was on average 6% lower than according to Timoshenko (Fig. 6). For specimens tested by forced vibrations, E′/γ was equivalent according to both theories, as was expected given their high slenderness (l/h = 75) (Nakao et al. 1985; Kubojima et al. 2004). These, however, displayed more variability (R2= 95% versus 99%) due to local variations.
2.5.3 Additional parameters to consider
The added mass of the thin steel piece fixed to the wooden test specimen has a negligible effect on tanδ, but decreases the
Fig. 3 Flowchart of the computer-driven vibration method developed (device II)
Fig. 2 Experimental devices: a wooden specimen; b supporting silk threads; c vibration node location; d thin steel plate; e electro-magnet. Device I: g eddy-current sensor facing a thin aluminium plate (f). Device II: h laser sensor
resonance frequency (Kataoka and Ono1975). Kubojima et al. (2005) calculated the change in the constant mn in the Euler–Bernouilli equation (Eq.1) due to the ratio (μ=M/m) of the added mass (M) to the mass of the wooden beam (m). For values of μ≤5% (approximately 0.7% in our experiments), this can be approached by linear relations. The resulting decrease in apparent E′/γ is of ≈−3.437×μ and was around −2.4% on average over all tested specimens. This effect could be neglected for dense woods, but it has to be corrected for very light ones, and subsequently must be taken into account when comparing in very different wood materials.
Supporting threads, when they are loose and flexible, have almost no influence on fR (Brancheriau and Baillères
2002) or on tanδ measurements, even if they are not strictly located at the position of the first mode’s node: An inaccuracy of ±5% of the total length should remain acceptable (Kataoka and Ono1975). Tight or stiff support-ing threads, however, may interfere with the specimen vibration and/or result in a coupling with the device’s frame
(Brancheriau et al.2010). Tanδ and fR are stable when the distance between the exciting electro-magnet and the steel piece is ≥2 mm, but measurements are affected when this distance is <1 mm (Kataoka and Ono 1975).
The fluid friction with air does not affect damping under the usual test conditions (Kataoka and Ono 1975; David 1999). In the low-frequency range (<100 Hz), however, its contribution would not be negligible for thin wooden beams (Kitahara and Matsumoto1973).
2.6 Data sorting and statistical analysis
Data were analysed at the specimen, wood type, and species levels. First, all tested specimens (N=1,792) were used for analysing the relationship between tanδ and E′/γ, by comparing present results with the“standard” trend from Ono and Norimoto (1983,1984):
tan dS¼ 10A ðE0=rÞB ð2Þ
where tanδS is “standard” damping coefficient and coef-ficients A and B are 1.23 and 0.68 over a wide range of softwoods (further detailed below in Sections3and 4).
Then, analyses of this relationship were detailed for three broad groups of normal wood: softwoods and hardwoods with low or high extractives content (EC). Classification into low (<5%) or high (>7%) EC was based on available database (e.g. Brémaud et al. 2010b) and/or literature values. Sapwood was usually considered as low EC unless contradictory data were known. Species with medium
Fig. 6 Comparison of E′/γ calculated according to Euler-Bernouilli (for small slender specimens in forced vibrations and bulk specimens in natural vibration) and to Timoshenko (for bulk specimens in natural vibration). Vertical error bars: standard deviation between 2 and 6 small specimens prepared from a bulk one
Fig. 5 Comparison of tanδ determined in the temporal (logarithmic decrement method) and frequency (bandwidth method) domains. Each point: average of three repetitions
Fig. 4 Range of variation ([max−min]/mean values) of tanδ between 3 to 6 repetitions per specimen, with different sensors and methods of determination
(5–7%) EC and species for which no information on EC could be obtained were excluded from this analysis, as were some samples with atypical heartwood. Specimens with important grain deviations were included in analyses of the tanδ–E′/γ relationship. However, these specimens were excluded from basic statistics on the different wood types, for which 1,317 specimens were kept as representative (see Table 1). Data were first averaged between different specimens from a given stock, then between the means of different stocks (when applicable).
The“deviation from standard damping”=DSδ (Brémaud 2006; Brémaud et al.2009,2010b) was used for expressing the “intrinsic viscosity” (i.e. de-correlated from specific modulus of elasticity) of the different wood types:
DSd¼ 100 tan di tan dS
tan dS ð3Þ
where tanδiis the damping coefficient of a given wood, and tanδSis the standard damping from Eq.2.
In order to compare all wood types according to various properties, principal component analysis (PCA) was per-formed, using XLstat® (Addinsoft SARL) in MS Excel. Active variables represented the three main aspects of specific gravity, elasticity and viscosity and were selected to be as far as possible de-correlated from each other. That is,“elasticity” was represented by E′/γ (instead of Young’s modulus E′, which is quite strongly correlated to specific gravity) and “viscosity” by DSδ (Eq. 3 above). The broad categories “softwoods”, “temperate hardwoods” and “tropical hard-woods” were added as inactive qualitative variables. 3 Results
3.1 Total diversity at the specimens’ level
Over all individual specimens, measured properties covered a continuous and broad range: 0.21–1.38 for specific gravity, 4.6–34.1 GPa for E′/γ, 3.3×10−3to 20.6×10−3for
tanδ (Table 1). Damping coefficient had the highest coefficient of variation (>40%), but the three properties covered a similar span (ratio between maximum and minimum values of 6–7).
Damping coefficient and specific modulus of elasticity followed a relationship very similar to the “standard” one (Eq. 2). This “standard” relationship was reported by Ono and Norimoto (1983, 1984) in the logarithmic representa-tion shown in Fig. 7, by plotting tanδ/(E′/γ) (which is supposed to be proportional to the energy dissipated per vibration cycle) versus E′/γ. This representation, however, reduces the apparent dispersion. When plotting directly tanδ versus E′/γ (as in Fig.8), the relationship has the form of a power law: tand ¼ 10A Eð 0=gÞB(i.e. linear regressions can be performed in a log-log scale, shown in the inset of Fig. 8). On all studied specimens of very different wood types, the relationship was highly significant (at a level< 0.1%: Pearson’s coefficient of correlation R=0.71, N=1,792), but explained only half of the variations in tanδ (R2
=0.5). This strength of association is of the same order as above references, when comparing the coefficients of determination (R2) obtained in the two different representations [i.e. by plotting tanδ directly, or tanδ/(E′/γ), versus E′/γ] (Table 2). Distinct categories—softwoods, hardwoods with low or high extractives content—showed lower dispersion (R2
=0.76, 0.73 and 0.57, respectively) and nearly parallel trends, but shifted towards higher or lower tanδ values (Fig.8). 3.2 Species diversity in vibrational properties
Considering the mean properties of normal heartwood from the different species (Table 3), the specific gravity (γ) ranged from 0.22 (Ceiba pentandra) to 1.31 (snakewood= Brosimum guianense); the specific storage modulus (E′/γ) from 9.0 GPa (Pinus caribeae) to 32.2 GPa (Picea sitchensis); and the damping coefficient (tanδ) from 3.9× 10−3 (Aniba canellila) to 18.7× 10−3 (Arbutus unedo). However, the widest range in E′/γ was observed when including reaction woods: from 6.3 GPa (compression
Table 1 Basic statistics of total diversity in specific gravity (γ), specific modulus of elasticity (E′/γ) and damping coefficient (tanδ), between specimens and between wood types
N γ E′/γ (GPa) tanδ (10−3)
Range Mean CV (%) Range Mean CV (%) Range Mean CV (%) Specimen level
All specimens 1,792 0.21–1.38 0.84 26 4.6–34.1 18.5 33 3.3–20.6 7.1 41 Representative of wood types 1,317 0.21–1.38 0.86 28 4.6–34.1 19.7 30 3.3–20.6 6.9 44 Wood type level
All wood types 98 0.22–1.31 0.81 31 6.3–32.7 20.0 32 3.9–18.7 7.7 42 Normal heartwood 78 0.22–1.31 0.83 30 9.0–32.2 20.0 29 3.9–18.7 7.4 43
wood of Pinus pinaster) to 32.7 GPa (tension wood from Populus sp.). The span in properties (ratio of maximum to minimum values) was 6.0 forγ, 4.8 for tanδ and 3.6 for E′/ γ (5.2 when including reaction wood). As previously observed at the specimen level, tanδ had the highest coefficient of variation between species (normal heartwood)
and between all wood types (Fig. 9; Table 1). On the contrary, within a given wood type, tanδ was a little less variable than E′/γ (mean coefficient of variation of 9% and 11%, respectively).
3.3 Principal components analysis on wood types
Principal components analysis allows representation of the diversity of wood types according to several properties. As active variables should be as independent as possible, the analysis was conducted on γ, E′/γ, and the deviation of damping from the standard tanδ–E′/γ trend (DSδ, Eq. 3). The Young’s modulus (E′), specific loss modulus
E00=g ¼ tand E0=g
ð Þ and damping coefficient (tanδ) were
projected as inactive variables (Fig.10a) in order to better understand the repartition of the individuals. Schematically, axis 1 mainly denotes “solidity” (high γ and E′, reflecting porosity of the cellular material), vertical axis 2 is principally governed by E′/γ (related to microfibril and/or grain angle), and the upper-left to lower-right diagonal expresses a decreasing viscous behaviour (DSδ and E″/γ), which is mostly related to chemical composition (Brémaud et al.2010b,2011c).
4.1 Interpretation of the tanδ−E′/γ relationship in terms of sources of variability between wood types
For hardwood specimens with low extractives content (EC), the relationship between tanδ and E′/γ had a R2
of 73% and constants A and B (Table2) nearly equal to the values of the “standard” relationship on softwoods (Ono and Norimoto 1983). The results in Ono and Norimoto (1983) are based on 25 species, which represent quite well different gymno-sperm families, whereas the present study had only 12 softwood species, which were mostly Pinaceae for which damping is usually higher than average (Brémaud et al.2009). Accordingly, the “softwood” trend here had slightly higher tanδ values than the “standard”, but was also slightly less dispersed (Table 2). Conversely, the hardwood relationship from Ono and Norimoto (1984) is much more dispersed (Table 2) and has slightly lower (≈−6%) tanδ than the “softwood standard”, probably because it includes several tropical species with high extractives content. The trend observed here on hardwood specimens with high EC (>7%) shows they clearly had a lower tanδ (−33% in average) at a given E′/γ, and a higher dispersion (R2
=57%), than both “standard softwoods” and hardwoods with low EC.
The relationship between tanδ and E′/γ is governed by the orientation of wood elements and can be reconstructed by models taking into account either the microfibril angle
Fig. 8 Relationships between tanδ and E′/γ for normal wood of softwoods and of hardwoods with low (<5%) or high (>7%) extractives content. The inset shows the logarithmic representation, which allows calculation of linear regressions
Fig. 7 Relationship between damping coefficient and specific dynamic modulus of elasticity: comparison of our global sampling with trends reported by Ono and Norimoto (1983,1984) by plotting tanδ/(E′/γ) versus E′/γ on log-log scale
(Obataya et al. 2000) or the grain angle (Brémaud et al. 2011b). Vertical shifts of curves can reflect differences in chemical composition (Obataya et al.2000; Brémaud et al. 2010a,2011a,c) and/or in wood moisture content (Obataya et al.1998; Sasaki et al.1988), both of which affect tanδ more than E′/γ. A shift in tanδ of approximately 30% was observed between the trend for normal wood and that for compression wood (species: spruce and pines) due to variations in lignin composition and structure (Brémaud et al. 2011c). Extractives, on the other hand, can either be neutral or decrease (or sometimes increase) tanδ by as much as a factor 2, while affecting only marginally the axial E′/γ (Brémaud et al. 2010a,b, 2011a; Matsunaga et al. 1996; Minato et al.1997,2010; Obataya et al.1999; Sakai et al. 1999; Yano1994; Yano et al.1995). This appears consistent with the important shift between the trends for hardwoods with low and high EC and with the high dispersion for the later. Extractives can also modify wood equilibrium moisture content (e.g. Hernandez2007) in a range of about 6–12% EMC at 20°C and 65%RH (Brémaud et al. 2010b), but moisture-related shifts in the tanδ-E′/γ trends mostly take place at higher wood MC (Sasaki et al.1988).
Thus, the“standard” relationship from Ono and Norimoto (1983) was confirmed by present results, both qualitatively (general form) and quantitatively (values of the constants A and B in Eq. 2, Table 2), and concerns, statistically, both representative softwoods and hardwoods with low extractive content. Deviations of damping coefficient of a given wood from this standard trend can be considered as a“normalised damping” (DSδ, Eq.3), relatively de-correlated from the effect of orientation, and mostly related to chemical variations.
4.2 Distribution of vibrational properties between broad categories
Globally, wood types were rather broadly distributed along the range of γ and E′/γ (Fig. 9a, d). Tropical hardwoods covered the whole range of specific gravity but with a
predominance of high values. Some of the studied soft-woods and temperate hardsoft-woods, however, were also denser than usual (normal wood of yew and compression woods of spruce and pines, secondary species of hardwoods withγ≥0.9). Softwoods (which included both compression wood, and the so-called “resonance wood” selected for string instruments soundboards) had the most scattered values of E′/γ. Tempered and tropical hardwoods were more distributed towards, respectively, lower and higher ranges of E′/γ. Consequently, together with their often high γ, Young’s modulus (E′, Fig.9b) higher than 20 GPa could only be found for tropical hardwoods. These were also the only category with very low (<6×10−3) tanδ (Fig.9e). This confirms that tropical hardwoods could not be replaced by temperate-zone species for applications requiring very low damping (e.g. xylophones) and/or high Young’s modulus (e.g. violin bows) (Holz 1996; Brémaud and Poidevin 2009; Brémaud 2012; Bucur 2006; Wegst 2006). The predominance of low tanδ for tropical hardwoods partly results from their often high values of E′/γ (as both properties are still correlated at the wood type level) and also from a lower intrinsic damping (DSδ, Fig.9f), which is mostly due to their often higher content of “mechanically active” extractive components (Brémaud et al.2010b). 4.3 Classification of wood types in relation to their origins and potential uses
In the PCA on all wood types, globally, a “continuum” of behaviour was observed, although the different wood catego-ries cover preferential areas (Fig.10b). The right-hand part of the “individuals” graph was characteristic of tropical hard-woods, in which some sub-groups may be defined. From a botanical point of view, the lower right corner (i.e. exceptionally low loss parameters and moderate E′/γ) was dominated by heartwood of species from certain genera (Dalbergia, Pterocarpus and Platymiscium) belonging to the Dalbergieae tribe (=dalbergioid clade,
Leguminosae-Table 2 Parameters of the relationshiptand ¼ 10A Eð 0=gÞBas obtained by regressions on different samples N specimens A B R2 direct tand ¼ f Eð 0=gÞ R2 combined tand= Eð 0=gÞ ¼ f Eð 0=gÞ All samples 1,792 1.322 0.692 0.50 0.86
Softwoods (normal wood=NW) 140 1.222 0.639 0.76 0.95 Hardwoods (NW) with high extractives content 1,153 1.474 0.620 0.57 0.90 Hardwoods (NW) with low extractives content 221 1.231 0.677 0.73 0.94 25 softwood speciesa 1,227 1.23 0.68 0.91 30 hardwood speciesb 118 1.34 0.62 0.83 Constants are derived from regressions based on E′/γ expressed in GPa.R2
directandR2combined=coefficient of determination obtained from plotting
tanδ directly versus E′/γ, or tanδ/(E′/γ) versus E′/γ, respectively
Table 3 Mean (m) values and coefficient of variation (CV=standard deviation/mean) of specific gravity (γ), specific storage modulus (E′/γ) and damping coefficient (tanδ) for normal heartwood of all studied species
Family Category Species Code N specimens N stocks γ E′/γ (GPa) tanδ (10−3)
m CV (%) m CV (%) m CV (%)
PINA S Abies alba Mill. Abi.al 4 1 0.54 4 30.0 5 6.7 4
ACER Te.H Acer pseudoplatanus L. Ace.ps 1 1 0.64 10.6 16.1
ACER Te.H Acer sp. (American) Ace.sp 1 1 0.72 10.5 11.5
CAES Tr.H Afzelia bipindensis Harms. Afz.bi 13 5 0.82 5 23.5 10 4.2 7 CAES Tr.H Afzelia quanzensis Welw. Afz.qu 5 1 0.85 7 12.7 5 11.1 16 LAUR Tr.H Aniba canelilla (Kunth) Mez Ani.ca 9 1 1.20 2 29.1 4 3.9 5
ERIC Te.H Arbutus unedo L. Arb.un 5 1 0.94 2 12.0 7 18.7 9
SAPO Tr.H Baillonella toxisperma Pierre Bai.to 6 1 0.83 1 21.2 3 7.2 4 PAPI Tr.H Bobgunnia fistuloides (Harms)
Kirkbr. & Wiersema
Bob.fi 19 2 0.96 5 17.3 10 4.8 8
PAPI Tr.H Bocoa prouacensis Aubl. Boc.pr 35 5 1.26 2 26.0 10 4.2 12 MORA Tr.H Brosimum guianense (Aubl.) Huber Bro.gu 41 11 1.31 2 22.5 7 5.4 10 MORA Tr.H Brosimum rubescens Taub. Bro.ru 39 7 0.99 6 23.3 11 4.5 8
MORA Tr.H Brosimum utile Pitt. Bro.ut 5 1 0.47 3 21.7 8 8.6 15
BUXA Te.H Buxus sempervirens L. Bux.se 6 2 0.93 0 9.6 12 15.3 9
CAES Tr.H Caesalpinia echinata Lam. Cae.ec 55 15 1.01 9 21.5 11 4.4 14
BETU Te.H Carpinus betulus L. Car.be 9 2 0.74 0 20.8 2 9.5 1
MELI Tr.H Cedrela odorata L. Ced.od 1 1 0.48 21.8 7.8
BOMB Tr.H Ceiba pentandra Gaertn. Cei.pe 5 1 0.22 10 10.1 13 14.0 12 CUPR S Chamaecyparis sp. (Hinoki) Cha.sp 14 1 0.39 3 27.0 7 6.3 6 LAUR Tr.H Chlorocardium rodiei (Schomb.) Rohwer Chl.ro 4 1 1.05 1 27.8 2 4.3 4
CORN Te.H Cornus mas L. Cor.ma 4 1 1.11 0 15.6 2 8.3 7
CUPR S Cupressus sempervirens L. Cup.se 11 3 0.49 13 17.1 17 8.9 19 PAPI Tr.H Dalbergia baronii Baker Dal.ba 14 1 0.75 3 19.4 8 5.2 7
PAPI Tr.H Dalbergia latifolia Roxb. Dal.la 1 1 0.75 18.5 7.3
PAPI Tr.H Dalbergia maritimensis or D. louvelli Dal.ma 5 2 1.07 10 21.0 2 4.0 17 PAPI Tr.H Dalbergia melanoxylon Guill. et Perr. Dal.me 10 2 1.31 1 15.7 12 5.8 14 PAPI Tr.H Dalbergia nigra (Vell.) Allemão ex Benth. Dal.ni 1 1 0.81 20.5 7.0
PAPI Tr.H Dalbergia retusa Hemsley Dal.re 1 1 0.95 11.8 8.6
PAPI Tr.H Dalbergia sp. (Bahia) Dal.sB 3 1 1.15 2 13.0 4 4.7 7
PAPI Tr.H Dalbergia sp. (Madagascar) Dal.sM 53 9 0.96 11 20.1 10 4.6 8 PAPI Tr.H Dalbergia sp. (Jacaranda do Para) Dal.sP 1 1 0.88 18.4 5.6 CAES Tr.H Dialium cochinchinense Pierre Dia.co 4 1 1.10 2 24.0 5 6.4 13 CAES Tr.H Dialium pachyphyllum Harms Dia.pa 12 2 1.01 13 26.3 6 6.2 8 EBEN Tr.H Diospyros sp. (Madagascar) Dio.sp 3 1 1.18 0 16.8 1 9.1 5 PAPI Tr.H Dipteryx odorata (Aubl.) Willd. Dip.od 9 1 0.99 3 16.4 2 5.9 3 CAES Tr.H Guibourtia arnoldiana J.Leon. Gui.ar 4 1 0.84 1 25.8 1 5.6 4 CAES Tr.H Guibourtia conjugata (Bolle) J. Léonard Gui.co 2 1 1.02 1 17.0 1 7.5 5
CAES Tr.H Guibourtia sp. Gui.sp 7 2 0.89 8 16.6 29 10.7 8
CAES Tr.H Hymenaea courbaril L. Hym.co 8 1 0.77 4 28.4 5 5.3 2
CAES Tr.H Hymenaea parvifolia Huber Hym.pa 9 1 1.11 2 23.4 5 5.0 1
JUGL Te.H Juglans nigra L. Jug.ni 1 1 0.58 12.7 8.0
MELI Tr.H Khaya senegalensis (Desr.) A. Juss. Kha.se 4 1 0.85 0 9.2 4 12.0 6 PAPI Te.H Laburnum anagyroides Medik. Lab.al 12 3 0.90 6 13.4 8 9.2 6 LAUR Tr.H Licaria cannella (Meisn.) Kosterm. Lic.ca 16 7 1.01 5 26.1 9 5.6 8 STER Tr.H Mansonia altissima (A. Chev.) A. Chev Man.al 4 1 0.62 4 21.4 9 5.7 5
MYRI Tr.H Mauloutchia sp. Mau.sp 5 1 0.71 1 26.6 8 7.7 7
PAPI Tr.H Millettia laurentii De Wild. Mil.la 9 1 0.93 2 23.3 3 4.8 6 CLUS Tr.H Moronobea coccinea Aubl. Mor.co 8 1 0.92 1 25.1 2 4.7 3
MORA Tr.H Morus mesozygia Stapf. Mor.me 3 1 0.87 2 19.3 7 5.1 1
PAPI Tr.H Ormosia flava (Ducke) Rudd Orm.fl 9 1 0.84 1 29.9 4 4.5 9 CAES Tr.H Peltogyne venosa (Vahl) Benth. Pel.ve 8 2 0.80 0 26.8 7 5.6 7
Papilionoideae). This is probably due to the characteristic nature of their extractives, which strongly decrease tanδ in several genera of this tribe (Yano et al.1995; Brémaud et al. 2009, 2010b, 2011a; Traoré et al. 2010). It also probably explains the predominance of Dalbergieae in the xylophone-making traditions of several continents (Brémaud2012; Holz 1996; Traoré et al.2010; Wegst2006). Still from the point of view of utilisations, woods currently used for making Baroque to Modern violin bows are grouped at the far end of axis 1, i.e. they are mainly described by their high specific gravity and Young’s modulus, along with a low tanδ (Brémaud and Poidevin 2009; Wegst 2006). Other wood types in their vicinity could consequently be considered for this application: We have proposed several promising alternative species to bow makers for conducting practical trials (to be published). Temperate hardwoods were generally rather distinct from tropical ones and dominated the lower left portion of the plane, i.e. woods characterised by their low modulus and high tanδ. Despite quite a wide range in specific
gravity, no clear multi-variable distinction appeared within this category, which might however simply reflect the moderate number (12) of species under study.
The only characteristic shared by all softwoods was their lower than average specific gravity. Their ordinary wood types were poorly differentiated according to vibrational properties. Nevertheless, a distinct sub-group including “lutherie-grade” Picea abies was primarily governed by high specific modulus of elasticity combined to proportion-ally high loss properties (DSδ and E″/γ). This group also comprised other species of Pinaceae, suggesting that “resonance” Norway spruce may not be unique in its vibrational properties. Old growth Sitka spruce is often used as“alternative resonance wood” (e.g. Ono and Norimoto 1983; Bucur2006), but the anatomical and chemical features of other woods of the same genus or even family could also lead to comparable properties (e.g. Brémaud2012).
When confronting species diversity with intra-specific variability, the sapwoods of hardwood species (both
Table 3 (continued)
Family Category Species Code N specimens N stocks γ E′/γ (GPa) tanδ (10−3)
m CV (%) m CV (%) m CV (%)
PINA S Picea abies Karst. Pic.ab 40 14 0.50 10 24.4 18 8.4 8
PINA S Picea sitchensis (Bong.) Carr. Pic.si 5 1 0.47 1 32.2 2 5.9 2
PINA S Pinus caribaea Morelet Pin.ca 3 1 0.36 4 9.0 2 13.2 3
PINA S Pinus nigra subsp. laricio Maire Pin.ni 5 1 0.51 4 19.2 6 8.8 6 PINA S Pinus patula Schiede ex. Schlecht. et Cham. Pin.pa 4 1 0.54 9 31.1 3 6.6 5
PINA S Pinus pinaster Aiton Pin.pi 18 7 0.42 6 14.2 12 12.0 10
PINA S Pinus sylvestris L. Pin.sy 14 5 0.48 12 17.9 14 10.6 13
PAPI Tr.H Platymiscium sp. Pla.sp 4 1 1.02 1 25.5 5 4.8 2
PAPI Tr.H Platymiscium ulei Harms Pla.ul 19 3 0.73 9 20.4 7 4.8 11
ROSA Te.H Prunus avium L. Pru.av 1 1 0.62 17.4 10.0
PAPI Tr.H Pterocarpus erinaceus Poir. Pte.er 86 4 0.83 3 19.3 4 5.6 6 PAPI Tr.H Pterocarpus macrocarpus Kurz Pte.ma 22 1 0.75 1 12.9 4 6.8 4 PAPI Tr.H Pterocarpus soyauxii Taub. Pte.so 170 16 0.77 9 18.3 15 5.2 14 PAPI Tr.H Pterocarpus tinctorius Welw. Pte.ti 6 1 0.93 2 14.0 7 6.8 9
ROSA Te.H Pyrus communis L. Pyr.co 4 1 0.69 3 9.9 9 16.7 11
RHIZ Tr.H Rhizophora mangle L. Rhi.ma 5 1 1.13 1 28.8 4 7.3 4
CAES Tr.H Scorodophloeus zenkeri Harms. Sco.ze 14 2 0.88 8 23.0 15 6.8 1
ROSA Te.H Sorbus domestica L. Sor.do 24 5 0.81 7 19.3 17 9.9 16
PAPI Tr.H Swartzia panacoco (Aubl.) Cowan Swa.pa 8 2 1.16 8 26.0 8 4.4 16
PAPI Tr.H Swartzia sp. Swa.sp 46 9 1.21 6 26.3 10 4.3 7
MELI Tr.H Swietenia macrophylla King Swi.ma 1 1 0.48 20.7 6.4
BIGN Tr.H Tabebuia sp. Tab.sp 4 1 0.85 1 23.2 4 5.0 2
TAXA S Taxus baccata L. Tax.ba 25 5 0.64 6 11.1 17 10.0 8
CUPR S Thuja plicata D.Don Thu.pl 1 1 0.39 19.5 7.2
RUTA Tr.H Zanthoxylum tsihanimposa H.Perr. Zan.ts 5 1 0.57 9 18.4 6 6.2 6 PAPI Tr.H Zollernia ilicifolia (Brongn.) Vogel
(or Swartzia sp.)
Zol.il 6 1 1.06 4 21.4 6 5.1 10
PAPI Tr.H Zollernia paraensis Huber Zol.pa 14 1 1.16 4 21.1 7 5.8 7
Botanical families are abbreviated by their four first letters S Softwoods, Te.H temperate hardwoods, Tr.H tropical hardwoods
temperate and tropical) covered a wide range of porosity and of E′/γ. However, they were distributed orthogonally to the“viscosity” direction, which meant they were “neutral” regarding DSδ and E″/γ. Regarding reaction wood, com-pression woods formed a small group with very low E′/γ (as expected) and also slightly negative DSδ (Brémaud et al.2011c). This group was not exceptional, however: It was
close to normal wood of yew and to some temperate hardwoods. The only tension wood under study (poplar) was completely the reverse, with a very high E′/γ and also exceptionally high normalised damping.
The multi-variate confrontation of all wood types suggests that: (1) species diversity is the biggest source of variation in specific gravity and Young’s modulus (with
Fig. 9 Distributions of specific gravity (a), dynamic mechanical properties (b–e) and “normalised damping” (f) for the 98 wood types
Fig. 10 Principal components analysis. a Projection of variables/ correlation circle. Solid lines Active variables (γ, E′/γ and DSδ); dashed lines inactive additional variables. b Projection of individuals.
Filled symbols Normal heartwood; open symbols normal sapwood; hatched symbols reaction wood. Labels: see Table 3; italics Dalber-gieae; underscored woods used for violin bows
reaction wood and heartwood formation as secondary effects); (2) reaction (compression or tension) wood formation is responsible for the most extreme differences in air-dry specific modulus of elasticity, ahead of the (nevertheless very large) inter-specific diversity; (3) taxonomy-related content in heartwood secondary metabo-lites appears to be the prominent source of diversity in normalised damping, although extreme variations in con-stitutive polymers (such as between normal and reaction woods) also play a significant role. These property-dependent responses to different sources of variability might have implications from a biomechanical point of view. Although present results concern air-dry wood properties, some tests on six tropical species suggest that little dispersed (but non-linear for damping) relationships can relate air-dry and green wood vibrational properties (Dlouhá2009; Dlouhá et al.2011).
From the viewpoint of acoustical end-uses, the present results allow better definition of the group characteristics of several preferred species for a given use in musical instruments making and to propose mechanically realistic alternative species. They also confirm that the traditional avoidance of sapwood in hardwoods and of compression wood in softwoods is justified, not only because of dimensional stability, aesthetical aspect or biological dura-bility, but mostly so because of vibrational characteristics. The very wide range of wood material studied also allowed identification of secondary, little-known species with high potential interest in selected acoustical end-uses. However, it should be kept in mind that, in order to compare very different wood types in a rigorous way, a well-defined and generalised methodology is required, as demonstrated in this paper.
Acknowledgements Authors thank P. Cabrolier and J. Dlouhá for conducting some tests; P. Détienne (CIRAD xylarium) for wood identification; C. Daigremont and S. Lotte (CIRAD workshop) and instrument makers, for providing wood material; and N. Poidevin for testing“new” woods for violin bows.
Funding This work has been supported by CNRS and CIRAD in France and by JSPS in Japan.
Bordonné PA (1989) Module dynamique et frottement intérieur dans le bois. Mesures sur poutres flottantes en vibrations naturelles. PhD, Institut National Polytechnique de Lorraine, Nancy Brancheriau L, Baillères H (2002) Natural vibration analysis of clear
wooden beams: a theoretical review. Wood Sci Technol 36:347–365 Brancheriau L, Kouchade C, Brémaud I (2010) Internal friction measurement of tropical species by various acoustic methods. J Wood Sci 56:371–379
Brémaud I (2006) Diversité des bois utilisés ou utilisables en facture d’instruments de musique. Doctorat, Université Montpellier II
Brémaud I (2012) Acoustical properties of wood in string instruments soundboards and tuned idiophones: biological and cultural diversity. J Acoust Soc Am 131. doi:10.1121/1.3651233
Brémaud I, Poidevin N (2009) Approches culturelles et mécaniques dans le choix des bois en facture: cas des archets anciens. In: 5th Conference on Interdisciplinary Musicology, CIM09, 26–29 Octobre 2009, Paris, France
Brémaud I, Minato K, Thibaut B (2009) Mechanical damping of wood as related to species classification: a preliminary survey. In: Thibaut B (ed) 6th Plant Biomechanics Conference PBM09, 16– 21 November 2009, Cayenne, French Guyana. pp 536–542 Brémaud I, Cabrolier P, Gril J, Clair B, Gérard J, Minato K, Thibaut B
(2010a) Identification of anisotropic vibrational properties of Padauk wood with interlocked grain. Wood Sci Technol 44:355–367 Brémaud I, Minato K, Langbour P, Thibaut B (2010b) Physico-chemical indicators of the inter-specific variability in vibration damping of wood. Ann For Sci 67:707
Brémaud I, Amusant N, Minato K, Gril J, Thibaut B (2011a) Effect of extractives on vibrational properties of African Padauk (Pterocarpus soyauxii Taub.). Wood Sci Technol 45:461–472
Brémaud I, Gril J, Thibaut B (2011b) Anisotropy of wood vibrational properties: dependence on grain angle and review of literature data. Wood Sci Technol 45:735–754
Brémaud I, Ruelle J, Thibaut A, Thibaut B (2011c) Changes in viscoelastic vibrational properties between compression and normal wood: roles of microfibril angle and of lignin. Holzfor-schung (submitted)
Bucur V (2006) Acoustics of wood. Springer, Berlin
Chave J, Coomes D, Jansen S, Lewis SL, Swenson NG, Zanne AE (2009) Towards a worldwide wood economics spectrum. Ecol Lett 12:351–366
David B (1999) Caractérisations acoustiques de structures vibrantes par mise en atmosphère raréfiée. PhD, Université Paris 6 Détienne P, Chanson B (1996) L’éventail de la densité du bois des
feuillus. Comparaison entre différentes régions du Monde. Bois For Trop 250:19–30
Dlouhá J (2009) Comportement viscoélastique longitudinal du bois vert: diversité et prédiction à long terme. Doctorat, Université Montpellier II
Dlouhá J, Alméras T, Clair B (2011) Representativeness of wood biomechanical properties measured after storage in different conditions. Trees. doi:10.1007/s00468-011-0636-9
Fukada E (1950) The vibrational properties of wood I. J Phys Soc Jpn 5:321–327
Hernandez RE (2007) Moisture sorption properties of hardwoods as affected by their extraneous substances, wood density, and interlocked grain. Wood Fiber Sci 39:132–145
Holz D (1996) Tropical hardwoods used in musical instruments—can we substitute them by temperate zone species? Holzforschung 50:121–129
Jones DIG (2001) Handbook of viscoelastic vibration damping. Wiley, Chichester
Kataoka A, Ono T (1975) The relations of experimental factors to the vibration and the measuring values of dynamic mechanical properties of wood. I. The experimental errors due to the measuring apparatus (in Japanese). Mokuzai Gakkaishi 21:543– 550
Kitahara R, Matsumoto T (1973) Mechanism of damping in wood (in Japanese). Mokuzai Gakkaishi 19:373–378
Kubojima Y, Ohtani T, Yoshihara H (2004) Effect of shear deflection on vibrational properties of compressed wood. Wood Sci Technol 38:237–244
Kubojima Y, Tonosaki M, Yoshihara H (2005) Effect of additional mass on the Young’s modulus of a wooden beam. J Test Eval 33:278–282
Matsunaga M, Sugiyama M, Minato K, Norimoto M (1996) Physical and mechanical properties required for violin bow materials. Holzforschung 50:511–517
Minato K, Sakai K, Matsunaga M, Nakatsubo F (1997) The vibrational properties of wood impregnated with extractives of some species of Leguminosae. Mokuzai Gakkaishi 43:1035– 1037
Minato K, Konaka Y, Brémaud I, Suzuki S, Obataya E (2010) Extractives of muirapiranga (Brosimun sp.) and its effects on the vibrational properties of wood. J Wood Sci 56:41–46
Nakao T, Okano T, Asano I (1985) Theoretical and experimental analysis of flexural vibration of the viscoelastic Timoshenko beam. J Appl Mech 52:728–731
Obataya E, Norimoto M (1995) Acoustic properties of cane (Arundo donax L.) used for reeds of woodwind instruments I. The relationships between vibrational properties and moisture content of cane (in Japanese). Mokuzai Gakkaishi 41:289–292
Obataya E, Norimoto M, Gril J (1998) The effects of adsorbed water on dynamic mechanical properties of wood. Polymer 39:3059–3064 Obataya E, Umezawa T, Nakatsubo F, Norimoto M (1999) The effects
of water-soluble extractives on the acoustic properties of reed (Arundo donax L.). Holzforschung 53:63–67
Obataya E, Ono T, Norimoto M (2000) Vibrational properties of wood along the grain. J Mater Sci 35:2993–3001
Obataya E, Minato K, Tomita B (2001) Influence of moisture content on the vibrational properties of hematoxylin-impregnated wood. J Wood Sci 47:317–321
Olsson AM, Salmén L (1992) Viscoelasticity of in situ lignin as affected by structure. Softwood vs. hardwood. In: ACS Sympo-sium Series No 489, Viscoelasticity of Biomaterials. American Chemical Society, pp 133–143
Olsson A-M, Salmén L (1997) The effect of lignin composition on the viscoelastic properties of wood. Nord Pulp Pap Res J 3:140–144 Ono T, Kataoka A (1979) The frequency dependence of the dynamic Young’s modulus and internal friction of wood used for the soundboard of musical Instruments II (in Japanese). Mokuzai Gakkaishi 25:535–542
Ono T, Norimoto M (1983) Study on Young’s modulus and internal friction of wood in relation to the evaluation of wood for musical instruments. Jpn J Appl Phys 22:611–614
Ono T, Norimoto M (1984) On physical criteria for the selection of wood for soundboards of musical instruments. Rheol Acta 23:652–656 Sakai K, Matsunaga M, Minato K, Nakatsubo F (1999) Effects of
impregnation of simple phenolics and natural polycyclic com-pounds on physical properties of wood. J Wood Sci 45:227–232 Sali S, Kopac J (1998) The influence of the different machining processes on the acoustic properties of wooden resonant boards. Catgut Acoust Soc J (II) 3:15–20
Sasaki T, Norimoto M, Yamada T, Rowell RM (1988) Effect of moisture on the acoustical properties of wood (in Japanese). Mokuzai Gakkaishi 34:794–803
Traoré B, Brancheriau L, Perré P, Stevanovic T, Diouf P (2010) Acoustic quality of vène wood (Pterocarpus erinaceus Poir.) for xylophone instrument manufacture in Mali. Ann For Sci 67:815 Wegst UGK (2006) Wood for sound. Am J Bot 93:1439–1448 Williamson BG, Wiemann MC (2010) Measuring wood specific
gravity… Correctly. Am J Bot 97:519–524
Yano H (1994) The changes in the acoustic properties of Western red cedar due to methanol extraction. Holzforschung 48:491–495 Yano H, Kyou K, Furuta Y, Kajita H (1995) Acoustic properties of
Brazilian rosewood used for guitar back plate (in Japanese). Mokuzai Gakkaishi 41:17–24